Incorporation of Fe3O4/CNTs nanocomposite in an epoxy coating for corrosion protection of carbon steel

In this study Fe3O4/CNTs composite with magnetic property was prepared by attaching magnetic nanoparticles (Fe3O4) to carbon nanotubes (CNTs) by hydrothermal method. The obtained Fe3O4/CNTs composite was characterized by Fourier transform infrared (FTIR) spectroscopy, powder x-ray diffraction and transmission electron microscopy. The Fe3O4/CNTs composite was then incorporated into an epoxy coating at concentration of 3 wt%. Corrosion protection of epoxy coating containing Fe3O4/CNTs composite was evaluated by electrochemical impedance spectroscopy and adhesion measurement. The impedance measurements show that Fe3O4/CNTs composite enhanced the corrosion protection of epoxy coating. The corrosion resistance of the carbon steel coated by epoxy coating containing Fe3O4/CNTs composite was significantly higher than that of carbon steel coated by clear epoxy coating and epoxy coating containing CNTs. FE-SEM photographs of fracture surface of coatings showed good dispersion of Fe3O4/CNTs composite in the epoxy matrix.


Introduction
Carbon nanotubes (CNTs) have excellent mechanical, electrical, magnetic, optical and thermal properties [1]. They are being studied for some special applications where high-performance materials are required and widely used as a reinforcing material in polymer matrix. In recent years, polymer composites reinforced with CNTs have attracted attention because CNTs enhance mechanical, electrical, thermal and morphological properties of the produced nanocomposite [2][3][4][5][6]. However, the fabrication of CNT-reinforced nanocomposites has two main problems: agglomeration of CNTs and weak interfacial interactions between the CNTs and matrix. To address these problems, many studies have proposed methods to uniformly disperse CNTs and enhance the interfacial interactions in the polymer matrix. The surface modification of CNTs is considered to improve the dispersion of CNTs in a polymer matrix.
Iron oxides such as magnetite, hematite, magnetite and goethite are commonly used as pigments for black, red, brown and yellow colors, respectively. They are widely used as active pigments in organic coatings due to their low cost, easy production and environmental acceptability and also as anticorrosive pigments [7,8].
In this study, composite nano-Fe 3 O 4 /carbon nanotubes (Fe 3 O 4 /CNTs) were prepared by hydrothermal method and characterized by Fourier transform infrared (FTIR) spectroscopy, powder x-ray diffraction and transmission electron microscopy. Corrosion protection performance of epoxy coatings containing Fe 3 O 4 /CNTs was evaluated by electrochemical impedance spectroscopy.

Experimental
The carbon nanotubes (CNTs) used were supplied by Institute of Materials Science, Vietnam Academy of Science and Technology. They were synthesized by catalytic carbon vapor deposition (CCVD) and had a purity of around 95%. The CNTs' diameter ranged from 15 to 90 nm. HNO 3 , FeCl 3 .6 H 2 O, FeSO 4 .7 H 2 O, KOH were purchased from Merck. The epoxy resin was an epoxy bisphenol A, YD-011X75. The hardener was an amine, Sunmide 307D-60. Both compounds were purchased from Kukdo and Air Poroducts and Chemicals.
CNTs were pretreated before the modification by the following procedure: 1 g of CNTs was dispersed in 100 ml of the nitric acid (65 wt%) in a 500 ml round bottom flask equipped with a condenser and the dispersion was refluxed under magnetic stirring for 48 h. The resulting dispersion was diluted in water and filtered. The resulting solid was washed up to neutral pH, and the sample was dried in vacuum at 40°C overnight.
Magnetite (Fe 3 O 4 ) was prepared by hydrothermal method (initial molar ratio Fe 2+ /Fe 3+ = 1/1). The precursor was mixed then transferred to a teflon-lined stainless steel bomb, 150 ml capacity, non-stirred autoclave and sealed (the as pre-hydrothermal process). The hydrothermal reaction was conducted in an oven for 7 h and temperatures 150°C. After reaction, the autoclave was naturally cooled to room temperature, then washed with distilled water and absolute alcohol to remove impurity ions. Nano-Fe 3 O 4 /carbon nanotubes composite (Fe 3 O 4 /CNTs) was synthesized using FeCl 3 .6H 2 O, FeSO 4 .7H 2 O, carbon nanotubes and KOH as starting materials using hydrothermal technique. Before each preparation of nano-Fe 3 O 4 /carbon nanotubes composite, the carbon nanotubes were refined in a solution conducted a main compound of HNO 3 acid. After that, the purified carbon nanotube was poured into a solution containing a mixture of iron salts and KOH solution. The precursors were mixed by the magnetic stirrer then transferred to a teflon-lined stainless steel bomb, 150 ml capacity, nonstirred autoclave and sealed. The hydrothermal reaction was conducted at 150°C for 7 h [9]. After reaction, the autoclave was naturally cool to room temperature. The solid was taken out of the Teflon autoclave, and then washed with distilled water and absolute alcohol to remove impurity ions.
The CNTs and Fe 3 O 4 /CNTs were incorporated into epoxy resin at concentration of 3 wt%. CNTs and Fe 3 O 4 / CNTs were dispersed in epoxy resin by ball mill for 24 h. The liquid paint was applied by spin coating and dried at ambient temperature for 24 h. The dry film thickness was about 20 μm (measured by a Minitest 600 Erichen digital meter).
Fourier transform infrared spectra were recorded with a Nexus 670 Nicolet spectrometer over the range 4000 cm −1 -400 cm −1 . X-ray diffraction (XRD) patterns were recorded on Siemens D5000 x-ray diffract meter with Cu-Kα radiation. Field emission scanning electron microscope (FE-SEM) observations were done by using a Hitachi S-4800.  For the electrochemical impedance spectroscopy (EIS) measurements, a three-electrode cell was used: the working electrode with an exposed area of 28 cm 2 , the saturated calomel reference electrode (SCE) and a platinum auxiliary electrode. The corrosive medium was a 0.5 M NaCl solution (reagent grade) in contact with air, quiescent and at ambient temperature. The electrochemical impedance measurements were performed using an Autolab PGStat30 over a frequency range of 100 kHz to 10 mHz with seven points per decade using 30 mV peak-to-peak sinusoidal voltage.

Intensity (a.u.)
The adhesion strength of the coatings on steel surface was determined by an adhesion tester PosiTest AT according to ASTM D4541.

Protection performance of coatings
The corrosion protection performance of coatings was evaluated by electrochemical impedance measurements.   coating, epoxy coating containing 3 wt% of CNTs, epoxy coating containing 3 wt% of Fe 3 O 4 and epoxy coating containing 3 wt% of Fe 3 O 4 /CNTs. After 7 days of immersion, the impedance diagram of epoxy coatings is characterized by one capacitive loop. The impedance diagrams of epoxy coatings containing CNTs, Fe 3 O 4 and Fe 3 O 4 /CNTs are characterized by two time constants, but the second time constant is not well defined. Electrochemical impedance diagram of an organic coating was interpreted as follows: the high-frequency (HF) part is related to the organic coating while the low-frequency (LF) part corresponds to the reactions occurring on the metal through defects and pores in the coatings [13,14]. The electrolyte permeation in the coatings is responsible for stabilizing the corrosion processes in the metallic substrate and for decreasing some of the mechanical and electrical properties of the coating. The resistance values associated with the HF part of epoxy coatings containing CNTs are higher and the resistance values associated with the HF part of epoxy coatings containing Fe 3 O 4 and Fe 3 O 4 /CNTs are lower than those obtained for pure epoxy coating.
After 70 days of immersion, the diagrams of coatings have different shapes, pure epoxy coatings have one time constant and the other coatings are characterized by two  It was proposed by Kittel et al and the group of Bierwagen that the impedance modulus at low frequencies (such as Z 1Hz or Z 10mHz ) measured versus exposure time could serve as an estimation of the corrosion protection of a painted metal [15][16][17][18]. The results obtained show that the presence of CNTs in epoxy coating improved the barrier properties of coating. However the effect of Fe 3 O 4 /CNTs is much higher than those of primary CNTs. Fe 3 O 4 /CNTs enhanced significantly the corrosion resistance of epoxy coatings.
The adhesion of coatings was determined and is presented in the table 1. By comparison with pure epoxy coatings, epoxy-coating-containing CNTs have significantly higher adhesion. The adhesion of coating containing Fe 3 O 4 is higher than the adhesion of epoxy coating, but lower than the adhesion of epoxy coating containing CNTs. The epoxy coatings containing Fe 3 O 4 /CNTs has the highest adhesion. The presence of Fe 3 O 4 /CNTs improved significantly the adhesion of epoxy coatings. These results are in agreement with the electrochemical impedance measurements.
FESEM images of the fracture surface of epoxy coating, epoxy coating containing 3 wt% of CNTs, epoxy coating containing 3 wt% of Fe 3 O 4 and epoxy coating containing 3 wt% of Fe 3 O 4 /CNTs are shown in figure 8.
It is observed that in the case of epoxy coating containing 3 wt% of Fe 3 O 4 , the Fe 3 O 4 particles are very well dispersed in epoxy. While in epoxy coating containing 3 wt% of CNTs, we can see the agglomeration of CNTs particles. There are the holes between the CNTs particles and epoxy matrix. In epoxy-coating-containing 3 wt% of Fe 3 O 4 /CNTs it can be seen that CNTs are well dispersed in epoxy matrix. The good dispersion of Fe 3 O 4 /CNTs in epoxy coatings can be explained by the interfacial interaction between Fe 3 O 4 /CNTs epoxy through the presence of Fe 3 O 4 on the CNTs surface.

Conclusion
Fe 3 O 4 /CNTs composite with magnetic property was successfully prepared by hydrothermal method. It was confirmed that the Fe 3 O 4 nanoparticles were adsorbed on the CNTs surface. The corrosion protection of carbon steel by an epoxy coatings containing Fe 3 O 4 /CNTs were investigated by electrochemical impedance spectroscopy. It was shown that the corrosion protection of the epoxy coatings was significantly higher in the presence of Fe 3 O 4 /CNTs by comparison with the pure epoxy coatings. The Fe 3 O 4 /CNTs composite improved significantly the adhesion of epoxy coatings on steel surface. FE-SEM revealed the better dispersion of Fe 3 O 4 /CNTs composite in epoxy matrix with CNTs particles.